alloys like Inconel 718 forms solid solutions that stabilize the γ' phase, which is crucial for enhancing high-temperature strength. The γ' phase, a nickel-aluminum compound, forms ordered precipitates that impede dislocation movement by acting as obstacles. These precipitates are coherent with the matrix and exhibit excellent thermal stability, meaning they resist coarsening even under prolonged thermal exposure. The alloy's ability to retain these finely dispersed γ' precipitates during thermal cycling is vital for maintaining its creep resistance. The presence of these particles prevents dislocations from bypassing them, ensuring that the material maintains its integrity under prolonged high-temperature exposure. The precise control of alloying elements and the aging process are critical to optimize the size and distribution of these precipitates, ensuring optimal creep resistance. For example, Inconel 718 is aged to develop γ' precipitates, which enhance its strength without losing its ductility. The aging process, involving specific temperature and time treatments, ensures the optimal formation of γ' precipitates, which are crucial for improving the alloy's resistance to creep. This process involves a controlled precipitation hardening treatment that optimizes the dispersion of γ' precipitates, which act as barriers to dislocation movement, thereby enhancing the alloy's creep resistance.

Precipitation hardening is another crucial mechanism in the design of superalloys, especially for enhancing their creep resistance. The aging process in these alloys induces the formation of fine, coherent precipitates within the matrix, which significantly strengthen the material. In Inconel 718, the presence of niobium and aluminum leads to the formation of γ' precipitates during aging. These ordered nickel-aluminum precipitates block dislocation movement by creating a barrier that prevents them from gliding through the matrix. The aging process in Inconel 718 stabilizes the γ' precipitates, making them more resistant to coarsening under thermal cycling. The formation of fine γ' precipitates is crucial for improving creep resistance. The size and distribution of these precipitates are tailored through aging treatments, which involve precise control over temperature and time. These precipitates not only increase the alloy's strength but also enhance its thermal stability, ensuring it can endure high-temperature exposure without losing its mechanical properties. The interaction between dislocations and these precipitates is such that they effectively block dislocations, thereby preventing them from moving through the crystal lattice. The control over aging processes is crucial for optimizing the formation of γ' precipitates, which is vital for maintaining the alloy's strength under long-term thermal exposure. The optimization of the aging treatment in Inconel 718 is achieved through controlled aging at temperatures that promote the formation of finely dispersed γ' precipitates, which are resistant to coarsening and contribute significantly to the alloy's creep resistance. These precipitates form a complex, three-dimensional network that blocks dislocation movement, making the alloy highly resistant to creep deformation under high temperatures.

Grain boundary strengthening is another essential mechanism that enhances the creep resistance of superalloys. The integrity of grain boundaries is critical for maintaining the material's strength at high temperatures. Alloying elements such as boron, zirconium, and titanium are added to form carbides and borides at grain boundaries. These particles pin the grain boundaries, making it more difficult for dislocations to move across them. In alloys like Haynes 230, boron and titanium are added to segregate at grain boundaries and form titanium-boride particles. These particles effectively immobilize dislocations, preventing them from moving along the grain boundaries—a significant creep mechanism at high temperatures. The presence of these grain boundary particles ensures the alloy maintains its strength over time, particularly under cyclic thermal conditions. These carbides and borides at grain boundaries serve as pinning points that prevent grain boundary sliding—a primary mechanism of creep deformation at high temperatures. The formation of these pinning particles significantly enhances the alloy's creep resistance by preventing dislocations from migrating along the grain boundaries, which is a critical feature for materials used in high-temperature applications. The Hall-Petch relationship describes the relationship between grain size and strength, showing that
the yield strength increases with a reduction in grain size due to grain boundary strengthening:

$$ \sigma_y = \sigma_0 + \frac{K}{\sqrt{d}} \qquad (314) $$

where $\sigma_y$ is the yield strength, $\sigma_0$ is the frictional stress, $K$ is a material constant, and $d$ is the average grain size. This equation quantitatively explains the role of grain boundaries in strengthening the alloy, demonstrating the effectiveness of grain boundary strengthening in preventing creep deformation. The segregation of elements such as boron and titanium at grain boundaries forms stable pinning phases that prevent dislocations from moving across these boundaries, thereby enhancing the alloy's creep resistance. This segregation not only increases the diffusional path length for atoms but also stabilizes the microstructure during thermal exposure, contributing significantly to the alloy's long-term strength and stability under high temperatures.

The presence of multiple phases in superalloys further contributes to their creep resistance. Advanced superalloys, like PWA 1480, contain a complex microstructure with $\gamma$, $\gamma'$, and $\gamma''$ phases. The $\gamma''$ phase, which is an ordered Ni3Nb phase, enhances the creep resistance by providing additional obstacles to dislocation motion. These $\gamma''$ precipitates act as barriers within the matrix, creating a more complex microstructure that enhances the alloy's high-temperature strength. The formation of these phases is controlled by alloy composition and heat treatment processes, which tailor the microstructure to optimize the alloy's creep resistance. The coherency strains introduced by $\gamma''$ precipitates are particularly effective at blocking dislocation movement, further stabilizing the microstructure during thermal cycling. These precipitates provide additional resistance to dislocation motion, thereby enhancing the creep strength of the superalloy, especially in applications requiring stable dimensional stability under thermal cycling.

To further justify these mechanisms, mathematical models and equations are employed to describe the creep behavior in superalloys. The Norton-Bailey creep law is one such model used to describe the creep strain rate:

$$ \dot{\epsilon} = A\sigma^n \exp\left(-\frac{Q}{RT}\right) \qquad (315) $$

where $\dot{\epsilon}$ is the creep strain rate, $\sigma$ is the applied stress, $A$ is a material constant related to the creep resistance, $n$ is the stress exponent, $Q$ is the activation energy for creep, $R$ is the gas constant, and $T$ is the absolute temperature. This equation encapsulates the combined effects of solid solution strengthening, precipitation hardening, and grain boundary strengthening. The stress exponent $n$ typically ranges from 3 to 5 for creep in superalloys, indicative of the dominant creep mechanisms such as dislocation glide, dislocation climb, and grain boundary sliding. The activation energy $Q$ reflects the energy barriers associated with dislocation movement and the stability of $\gamma'$ precipitates. The effectiveness of superalloy compositions in enhancing creep resistance can be quantitatively described by these equations, providing a predictive tool for the development of new superalloys. The Norton-Bailey model effectively combines the effects of all the mechanisms discussed, illustrating how they contribute to the creep resistance of superalloys. These equations serve as a powerful tool for predicting the performance of superalloys under various service conditions, providing valuable insights into the development of advanced materials for high-temperature applications.

In conclusion, the prevention of creep in superalloys involves a complex interplay of mechanisms such as solid solution strengthening, precipitation hardening, grain boundary strengthening, and the presence of multiple phases. The precise control of alloy composition, microstructure, and heat treatment processes is critical for the development of superalloys that maintain their mechanical properties over extended periods at high temperatures. The ongoing research in this field aims to further refine these mechanisms, enabling the development of new superalloys with even higher creep resistance, improved thermal stability, and extended operational lifetimes. These advancements are
essential for high-performance applications in aerospace, power generation, and other industries requiring materials that can operate under extreme conditions.

# 13 Famous Accidents

## 13.1 Big Dig tunnel ceiling collapse in Boston on July 2006

The catastrophic collapse of the Big Dig tunnel ceiling in Boston, Massachusetts, in July 2006, has been attributed in significant part to the phenomenon of creep in the epoxy anchor adhesive used to secure the ceiling panels [108]. This tragic failure underscores the critical importance of understanding the time-dependent behavior of materials under sustained loads, particularly in safety-critical applications. Epoxy adhesives, while often chosen for their strong initial bonding properties and resistance to environmental degradation, are inherently viscoelastic materials. This viscoelasticity means they exhibit both elastic (recoverable) and viscous (time-dependent) deformation characteristics when subjected to stress. Under sustained loads, such as the weight of ceiling panels in the Big Dig tunnel, creep deformation can occur as the material undergoes gradual and irreversible elongation or deformation over time. In the case of the Big Dig, the epoxy adhesive was used to anchor bolts that supported the heavy concrete ceiling panels. Over time, and under the constant tensile load exerted by the weight of these panels, the adhesive likely experienced progressive creep, which diminished its load-carrying capacity. The viscoelastic nature of epoxy adhesives makes them particularly susceptible to creep at elevated temperatures, even within ranges considered normal for the operational environment. However, even in the absence of significant temperature fluctuations, the prolonged application of stress can lead to molecular reorganization within the adhesive, reducing its mechanical integrity. In this instance, the adhesive's gradual deformation under the sustained load may have resulted in the bolts slipping or detaching entirely, thereby undermining the overall structural stability of the ceiling. Compounding this issue is the possibility that the design and material selection did not fully account for the long-term creep behavior of the adhesive under the specific loading conditions. This failure to anticipate or mitigate creep may have been due to an underestimation of the stresses involved, a lack of rigorous long-term testing of the adhesive under simulated conditions, or an overreliance on the initial strength properties of the material without adequate consideration of its time-dependent degradation. The collapse of the ceiling panels, tragically resulting in loss of life and severe damage, illustrates the dire consequences of overlooking creep in the design and maintenance of critical infrastructure. This event has since prompted greater scrutiny of material selection, design practices, and quality control in construction projects, emphasizing the need for thorough testing and analysis of all materials used, particularly those subjected to sustained loads in safety-critical applications. Furthermore, it highlights the importance of incorporating redundancy and fail-safe mechanisms in structural designs to prevent catastrophic failures even in the event of material degradation. The Big Dig incident serves as a stark reminder of the complex interplay between material properties, environmental conditions, and structural demands, emphasizing the necessity for rigorous engineering practices to ensure long-term safety and reliability.

## 13.2 Collapse of the World Trade Center on September 11, 2001

The collapse of the World Trade Center, while primarily attributed to the significant reduction in yield strength of structural materials at elevated temperatures, also involved the critical contribution of creep deformation caused by the extreme thermal conditions during the event. The structural steel within the towers was subjected to extraordinarily high temperatures due to the intense and sustained fires following the impact of the airplanes. At these elevated temperatures, steel experiences a marked decline in its ability to withstand stress, as the temperature-induced softening reduces its yield strength, which is the stress level at which a material begins to deform plastically. Beyond this thermal softening, creep became a critical factor under these conditions because the steel components were subjected to both sustained mechanical loads from the weight of the building and the additional
thermal stress caused by the uneven heating. Creep in metals, including structural steel, is characterized by time-dependent plastic deformation under constant stress, and its effects become pronounced at high temperatures, particularly above approximately 0.4 times the material's melting temperature (in Kelvin). In the case of the World Trade Center, the extreme heat likely exceeded this threshold, accelerating creep deformation. The steel beams and columns, which were essential to maintaining the structural integrity of the towers, experienced gradual elongation and deformation due to creep. This deformation compromised the load-bearing capacity of the steel elements, leading to progressive failures within the structural framework. As the steel components deformed, the redistribution of loads caused additional stresses on already weakened elements, creating a cascade effect that further destabilized the structure. The combined effects of reduced yield strength and accelerated creep led to significant deformations, particularly in the connections between beams and columns, which were critical for structural stability. These deformations likely caused the misalignment of key load paths and the failure of essential joints, which are critical points in the structural network that rely on precise alignment and material strength to function effectively. As these elements failed under the combined effects of creep and thermal softening, the structural system of the towers could no longer support the immense gravitational forces of the upper floors. This ultimately led to the rapid and catastrophic collapse of the towers. The role of creep in this scenario underscores the importance of considering time-dependent deformation in the design and analysis of structures subjected to high-temperature conditions, especially in situations involving fire or other extreme heat sources. It also highlights the complex interplay between thermal effects, material behavior, and structural stability during high-temperature events, emphasizing the necessity for advanced modeling and simulation to predict and mitigate such catastrophic failures in future designs [109].

# 14 Conclusions

This rigorous analysis of creep deformation integrates mechanistic insights and phenomenological descriptions into a comprehensive framework. By coupling diffusion kinetics, dislocation motion, and damage mechanics, the models presented herein provide a robust foundation for predicting and mitigating time-dependent deformation.

# 15 Acknowledgments

The authors acknowledge the contributions of researchers whose foundational work has shaped our understanding of creep deformation.

# References

[1] Kassner, M. E. (2015). Fundamentals of creep in metals and alloys. Butterworth-Heinemann. https://www.sciencedirect.com/book/9780080994277/fundamentals-of-creep-in-metals-and-alloys

[2] Poirier, J. P. (1985). Creep of crystals: high-temperature deformation processes in metals, ceramics and minerals. Cambridge University Press. https://www.cambridge.org/core/books/creep-of-crystals/6DAEE35A6BAD29EC9D067C4DAA48177B

[3] Penny, R. K., and Marriott, D. L. (2012). Design for creep. Springer Science and Business Media. https://link.springer.com/book/10.1007/978-94-011-0561-3

[4] Naumenko, K., and Altenbach, H. (2007). Modeling of creep for structural analysis. Springer Science and Business Media. https://link.springer.com/book/10.1007/978-3-540-70839-1
[5] Boyle, J. T., and Spence, J. (2013). Stress analysis for creep. Elsevier. https://www.sciencedirect.com/book/9780408011723/stress-analysis-for-creep

[6] Ashby, M. F., and Jones, D. R. (2012). Engineering materials 1: an introduction to properties, applications and design (Vol. 1). Elsevier. https://shop.elsevier.com/books/engineering-materials-1/jones/978-0-08-096665-6

[7] Frost, Harold J.; Ashby, Michael F. (1982). Deformation-Mechanism Maps: The Plasticity and Creep of Metals and Ceramics. Pergamon Press. ISBN 978-0-08-029337-0. https://defmech.engineering.dartmouth.edu/

[8] Turner, S. (2001). Creep of polymeric materials. Encyclopedia of materials: science and technology, 1813-1817. https://www.sciencedirect.com/science/article/abs/pii/B0080431526003284?via%3Dihub

[9] Passmore, E. M., Duff, R. H., and Vasilos, T. (1966). Creep of dense, polycrystalline magnesium oxide. Journal of the American Ceramic Society, 49(11), 594-600. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1966.tb13175.x

[10] Tremper, R. T., and Gordon, R. S. (1971). Effect of nonstoichiometry on the viscous creep of iron-doped polycrystalline magnesia (No. COO-1591-15; UTEC-MSE-71-102; CONF-711030-8). Utah Univ., Salt Lake City. Div. of Materials Science and Engineering. https://www.osti.gov/servlets/purl/4717607

[11] Vandervoort, R. R., and Barmore, W. L. (1963). Compressive creep of polycrystalline beryllium oxide. Journal of the American Ceramic Society, 46(4), 180-184. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1963.tb11711.x

[12] Hollenberg, G. W., and Gordon, R. S. (1973). Effect of oxygen partial pressure on the creep of polycrystalline Al2O3 doped with Cr, Fe, or Ti. Journal of the American Ceramic Society, 56(3), 140-147. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1973.tb15430.x

[13] Ahres, T. J. (1995). Rock Physics and Phase Relations a handbook of physical constants: Washington. American Geophysical Union, 190-191. https://www.wiley.com/en-us/Rock+Physics+and+Phase+Relations%3A+A+Handbook+of+Physical+Constants-p-9781118668108

[14] Berry, J., Rottler, J., Sinclair, C. W., and Provatas, N. (2015). Atomistic study of diffusion-mediated plasticity and creep using phase field crystal methods. Physical Review B, 92(13), 134103. https://journals.aps.org/prb/abstract/10.1103/PhysRevB.92.134103

[15] Goldsby, D. L. (2006). Superplastic flow of ice relevant to glacier and ice-sheet mechanics. Glacier science and environmental change, 308-314. https://onlinelibrary.wiley.com/doi/abs/10.1002/9780470750636.ch60

[16] Courtney, T. H. (2005). Mechanical behavior of materials. Waveland Press. https://www.waveland.com/browse.php?t=394

[17] Nabarro, F. R. N. (1948). Deformation of crystals by the motion of single ions. Report of a Conference on Strength of Solids, Physical Society, London, 75-90. https://cir.nii.ac.jp/crid/1370004233292144776

[18] Herring, C. (1950). Diffusional viscosity of a polycrystalline solid. Journal of applied physics, 21(5), 437-445. https://pubs.aip.org/aip/jap/article/21/5/437/159377/Diffusional-Viscosity-of-a-Polycrystalline-Solid
[19] Neu, R. W., and Sehitoglu, H. (1989). Thermomechanical fatigue, oxidation, and creep: Part I. Damage mechanisms. *Metallurgical transactions A*, 20, 1755-1767. https://link.springer.com/article/10.1007/BF02663207

[20] Neu, R. W., and Sehitoglu, H. (1989). Thermomechanical fatigue, oxidation, and creep: Part II. Life prediction. *Metallurgical transactions A*, 20, 1769-1783. https://link.springer.com/article/10.1007/BF02663208

[21] Meyers, M. A., and Chawla, K. K. (2008). Mechanical behavior of materials. Cambridge university press. https://www.cambridge.org/highereducation/books/mechanical-behavior-of-materials/48AD6E15E989D76D5DAF9926123137CF?chapterId=CB09780511810947A169

[22] Coble, R. L. (1963). A model for boundary diffusion controlled creep in polycrystalline materials. *Journal of applied physics*, 34(6), 1679-1682. https://pubs.aip.org/aip/jap/article/34/6/1679/362784/A-Model-for-Boundary-Diffusion-Controlled-Creep-in

[23] Cottrell, A. H., and Jaswon, M. A. (1949). Distribution of solute atoms round a slow dislocation. *Proceedings of the Royal Society of London. Series A. Mathematical and Physical Sciences*, 199(1056), 104-114. https://www.jstor.org/stable/98371

[24] Cottrell, A. H. (1953). LXXXVI. A note on the Portevin-Le Chatelier effect. The London, Edinburgh, and Dublin Philosophical Magazine and Journal of Science, 44(355), 829-832. https://www.tandfonline.com/doi/abs/10.1080/14786440808520347

[25] Gibbs, G.B. (1966), Grain Boundary Impurity Diffusion. phys. stat. sol. (b), 16: K27-K29. https://doi.org/10.1002/pssb.19660160143, https://onlinelibrary.wiley.com/doi/10.1002/pssb.19660160143

[26] Wei, Y., Bower, A. F., & Gao, H. (2010). Analytical model and molecular dynamics simulations of the size dependence of flow stress in amorphous intermetallic nanowires at temperatures near the glass transition. *Physical Review B—Condensed Matter and Materials Physics*, 81(12), 125402. https://journals.aps.org/prb/abstract/10.1103/PhysRevB.81.125402

[27] Penning, P. (1972). Mathematics of the portevin-le chatelier effect. *Acta Metallurgica*, 20(10), 1169-1175. https://www.sciencedirect.com/science/article/pii/0001616072901654

[28] Yilmaz, A. (2011). The Portevin–Le Chatelier effect: a review of experimental findings. *Science and technology of advanced materials*, 12(6), 063001. https://www.tandfonline.com/doi/full/10.1088/1468-6996/12/6/063001

[29] Rizzi, E., and Hähner, P. (2004). On the Portevin–Le Chatelier effect: theoretical modeling and numerical results. *International Journal of Plasticity*, 20(1), 121-165. https://www.sciencedirect.com/science/article/pii/S0749641903000354?via%3Dihub

[30] Jiang, H., Zhang, Q., Chen, X., Chen, Z., Jiang, Z., Wu, X., and Fan, J. (2007). Three types of Portevin–Le Chatelier effects: Experiment and modelling. *Acta materialia*, 55(7), 2219-2228. https://www.sciencedirect.com/science/article/pii/S1359645406007543?via%3Dihub

[31] Burton, B. (1982). The influence of solute drag on dislocation creep. *Philosophical Magazine A*, 46(4), 607-616. https://www.tandfonline.com/doi/abs/10.1080/01418618208236916

[32] Heald, P. T., and Harbottle, J. E. (1977). Irradiation creep due to dislocation climb and glide. *Journal of Nuclear Materials*, 67(1-2), 229-233. https://www.sciencedirect.com/science/article/pii/0022311577901775
[33] Mansur, L. K. (1979). Irradiation creep by climb-enabled glide of dislocations resulting from preferred absorption of point defects. Philosophical Magazine A, 39(4), 497-506. https://www.tandfonline.com/doi/abs/10.1080/01418617908239286

[34] Weertman, J. (1957). Steady-state creep of crystals. Journal of Applied Physics, 28(10), 1185-1189. https://pubs.aip.org/aip/jap/article/28/10/1185/161881/Steady-State-Creep-of-Crystals

[35] Mott, N. F. (1955). Dislocations, work-hardening and creep. Nature, 175, 365-367. https://doi.org/10.1038/175365a0, https://www.nature.com/articles/175365a0

[36] Harper, J., and Dorn, J. E. (1957). Viscous creep of aluminum near its melting temperature. Acta Metallurgica, 5(11), 654-665. https://www.sciencedirect.com/science/article/pii/0001616057901128

[37] Mohamed, F. A., Murty, K. L., and Morris, J. W. (1973). Harper-Dorn creep in al, pb, and sn. Metallurgical Transactions, 4, 935-940. https://link.springer.com/article/10.1007/BF02645593

[38] Sousa, J. R., & Ghosh, S. (2025). A New Generalization of the Riemann Functional Equation.

[39] Barrett, C. R., Muehleisen, E. C., and Nix, W. D. (1972). High temperature-low stress creep of Al and Al+ 0.5 Fe. Materials Science and Engineering, 10, 33-42. https://www.sciencedirect.com/science/article/pii/0025541672900638

[40] Kassner, M. E., and Pérez-Prado, M. T. (2000). Five-power-law creep in single phase metals and alloys. Progress in materials science, 45(1), 1-102. https://www.sciencedirect.com/science/article/pii/S0079642599000067

[41] Singh, S. P., Kumar, P., and Kassner, M. E. (2020). The low-stress and high-temperature creep in LiF single crystals: An explanation for the So-called Harper-Dorn creep. Materialia, 13, 100864. https://www.sciencedirect.com/science/article/pii/S2589152920302805

[42] Srivastava, V., McNee, K. R., Jones, H., and Greenwood, G. W. (2005). Tensile creep behaviour of coarse grained copper foils at high homologous temperatures and low stresses. Materials science and technology, 21(6), 701-707. https://www.tandfonline.com/doi/abs/10.1179/174328405X46105

[43] Malakondaiah, G., and Rao, P. R. (1979). Grain size independent viscous creep in alpha titanium and beta cobalt. Scripta Metallurgica, 13(12), 1187-1190. https://www.sciencedirect.com/science/article/pii/0036974879902801

[44] Blum, W., and Maier, W. (1999). Harper-Dorn Creep—a Myth?. physica status solidi (a), 171(2), 467-474. https://onlinelibrary.wiley.com/doi/abs/10.1002/%28SICI%291521-396X%28199902%29171%3A2%3C467%3A%3AAID-PSSA467%3E3.0.CO%3B2-8

[45] Ginter, T. J., Chaudhury, P. K., and Mohamed, F. A. (2001). An investigation of Harper-Dorn creep at large strains. Acta materialia, 49(2), 263-272. https://www.sciencedirect.com/science/article/pii/S1359645400003165

[46] Ginter, T. J., and Mohamed, F. A. (2002). Evidence for dynamic recrystallization during Harper-Dorn creep. Materials Science and Engineering: A, 322(1-2), 148-152. https://www.sciencedirect.com/science/article/pii/S0921509301011273

[47] McClay, K. R. (1977). Pressure solution and Coble creep in rocks and minerals: a review. Journal of the Geological Society, 134(1), 57-70. https://www.lyellcollection.org/doi/abs/10.1144/gsjgs.134.1.0057
[48] Wheeler, J. (1992). Importance of pressure solution and coble creep in the deformation of polymineralic rocks. Journal of Geophysical Research: Solid Earth, 97(B4), 4579-4586. https://agupubs.onlinelibrary.wiley.com/doi/abs/10.1029/97JB02476

[49] Blum, W., and Eisenlohr, P. (2009). Dislocation mechanics of creep. Materials Science and Engineering: A, 510, 7-13. https://www.sciencedirect.com/science/article/pii/S0921509308014123

[50] Hirth, G., and Tullis, J. A. N. (1992). Dislocation creep regimes in quartz aggregates. Journal of structural geology, 14(2), 145-159. https://www.sciencedirect.com/science/article/abs/pii/019181419290053Y

[51] Somekawa, H., Hirai, K., Watanabe, H., Takigawa, Y., and Higashi, K. (2005). Dislocation creep behavior in Mg-Al-Zn alloys. Materials Science and Engineering: A, 407(1-2), 53-61. https://www.sciencedirect.com/science/article/pii/S0921509305006696

[52] Renner, J., Evans, B., and Siddiqi, G. (2002). Dislocation creep of calcite. Journal of Geophysical Research: Solid Earth, 107(B12), ECV-6. https://agupubs.onlinelibrary.wiley.com/doi/full/10.1029/2001JB001680

[53] Pollock, T. M., and Argon, A. S. (1992). Creep resistance of CMSX-3 nickel base superalloy single crystals. Acta Metallurgica et Materialia, 40(1), 1-30. https://www.sciencedirect.com/science/article/pii/095671519290195K

[54] Kakehi, K. (2000). Effect of primary and secondary precipitates on creep strength of Ni-base superalloy single crystals. Materials Science and Engineering: A, 278(1-2), 135-141. https://www.sciencedirect.com/science/article/pii/S0921509399005791

[55] Sun, F., Gu, Y. F., Yan, J. B., Xu, Y. X., Zhong, Z. H., and Yuyama, M. (2016). Creep deformation and rupture mechanism of an advanced wrought NiFe-based superalloy for 700° C class A-USC steam turbine rotor application. Journal of Alloys and Compounds, 687, 389-401. https://www.sciencedirect.com/science/article/pii/S0925838816318448

[56] Zhang, J. X., Murakumo, T., Harada, H., Koizumi, Y., and Kobayashi, T. (2004). Creep deformation mechanisms in some modern single-crystal superalloys. Superalloys, 2004, 189-195. https://www.tms.org/Superalloys/10.7449/2004/Superalloys_2004_189_195.pdf

[57] Ghosh, S. (2024). Tensor Derivative in Curvilinear Coordinates. https://engrxiv.org/ preprint/view/4210

[58] Zhang, J. X., Murakumo, T., Harada, H., and Koizumi, Y. J. S. M. (2003). Dependence of creep strength on the interfacial dislocations in a fourth generation SC superalloy TMS-138. Scripta Materialia, 48(3), 287-293. https://www.sciencedirect.com/science/article/pii/S1359646202003792?via%3Dihub

[59] Ennis, P. J., and Czyrska-Filemonowicz, A. (2003). Recent advances in creep-resistant steels for power plant applications. Sadhana, 28, 709-730. https://link.springer.com/article/10.1007/BF02706455

[60] Pekguleryuz, M., and Celikin, M. (2010). Creep resistance in magnesium alloys. International Materials Reviews, 55(4), 197-217. https://www.tandfonline.com/doi/abs/10.1179/095066010X12646898728327

[61] Mo, N., Tan, Q., Bermingham, M., Huang, Y., Dieringa, H., Hort, N., and Zhang, M. X. (2018). Current development of creep-resistant magnesium cast alloys: A review. Materials and Design, 155, 422-442. https://www.sciencedirect.com/science/article/pii/S0264127518304982?via%3Dihub
[62] Darling, K. A., Rajagopalan, M., Komarasamy, M., Bhatia, M. A., Hornbuckle, B. C., Mishra, R. S., and Solanki, K. N. (2016). Extreme creep resistance in a microstructurally stable nanocrystalline alloy. *Nature*, **537**(7620), 378-381. https://pubmed.ncbi.nlm.nih.gov/27629642/

[63] Yang, J., Zhang, Z., Friedrich, K., and Schlarb, A. K. (2007). Creep resistant polymer nanocomposites reinforced with multiwalled carbon nanotubes. *Macromolecular rapid communications*, **28**(8), 955-961. https://onlinelibrary.wiley.com/doi/full/10.1002/marc.200600866

[64] Bell, R. L., and Langdon, T. G. (1967). An investigation of grain-boundary sliding during creep. *Journal of Materials Science*, **2**, 313-323. https://link.springer.com/article/10.1007/BF00572414

[65] Rachinger, W. A. (1956). Glide in lead telluride. *Acta Metallurgica*, **4**(6), 647-649. https://www.sciencedirect.com/science/article/pii/0001616056901699

[66] Lifshitz, I. M. (1963). On the theory of diffusion-viscous flow of polycrystalline bodies. *Sov. Phys. Jetp-USSR*, **17**(4), 909. http://www.jetp.ras.ru/cgi-bin/dn/e_017_04_0909.pdf

[67] Raj, R., and Ashby, M. F. (1971). On grain boundary sliding and diffusional creep. *Metallurgical transactions*, **2**, 1113-1127. https://link.springer.com/article/10.1007/BF02664244

[68] Kingery, W. D., & Berg, M. (1955). Study of initial stages of sintering solids by viscous flow, evaporation-condensation, and self-diffusion. *Journal of Applied Physics*, **26**(10), 1205-1212. https://doi.org/10.1063/1.1721874, https://pubs.aip.org/aip/jap/article/26/10/1205/160664/Study-of-the-Initial-Stages-of-Sintering-Solids-by

[69] Ashby, M. F. (1972). A first report on deformation-mechanism maps. *Acta Metallurgica*, **20**(7), 887-897. https://doi.org/10.1016/0001-6160(72)90082-X, https://www.sciencedirect.com/science/article/pii/000161607290082X

[70] Bhaduri, A. (2018). Mechanical properties and working of metals and alloys (Vol. 264). Singapore: Springer Singapore. https://link.springer.com/book/10.1007/978-981-10-7209-3

[71] Balluffi, R. W., Allen, S. M., & Carter, W. C. (2005). Kinetics of materials. John Wiley & Sons.

[72] Langdon, T. G. (2006). Grain boundary sliding revisited: Developments in sliding over four decades. *Journal of Materials Science*, **41**, 597-609. https://link.springer.com/article/10.1007/s10853-006-6476-0

[73] Langdon, T. G. (2013). Twenty-five years of ultrafine-grained materials: Achieving exceptional properties through grain refinement. *Acta Materialia*, **61**(19), 7035-7059. https://www.sciencedirect.com/science/article/pii/S1359645413006149

[74] Schiøtz, J., & Jacobsen, K. W. (2003). A maximum in the strength of nanocrystalline copper. *Science*, **301**(5638), 1357-1359. https://www.science.org/doi/full/10.1126/science.1086636

[75] Yamakov, V., Wolf, D., Phillpot, S. R., & Gleiter, H. (2002). Grain-boundary diffusion creep in nanocrystalline palladium by molecular-dynamics simulation. *Acta Materialia*, **50**(1), 61-73. https://www.sciencedirect.com/science/article/pii/S1359645401003299

[76] Caro, A., Farkas, D., Bringa, E. M., Gilmer, G. H., & Zepeda-Ruiz, L. A. (2010, February). Effects of microalloying on the mobility and mechanical response of interfaces in nanocrystalline Cu. In *Materials Science Forum* (Vol. 633, pp. 21-30). Trans Tech Publications Ltd. https://www.scientific.net/MSF.633-634.21
[77] Yang, X., Li, J., & Wang, P. (2020). Grain boundary migration in nanocrystalline Ni under constant shear strains and its mechanism. Computational Materials Science, 176, 109530. https://www.sciencedirect.com/science/article/pii/S0927025620300215

[78] Van Swygenhoven, H., Caro, A., & Farkas, D. (2001). A molecular dynamics study of polycrystalline fcc metals at the nanoscale: grain boundary structure and its influence on plastic deformation. Materials Science and Engineering: A, 309, 440-444. https://www.sciencedirect.com/science/article/pii/S0921509300017949

[79] Schiotz, J., Vegge, T., & Jacobsen, K. W. (1998). Atomic-scale modeling of the deformation of nanocrystalline metals. MRS Online Proceedings Library (OPL), 538, 299. https://www.cambridge.org/core/journals/mrs-online-proceedings-library-archive/article/atomicscale-modeling-of-the-deformation-of-nanocrystalline-metals/39D96AE2881B141C423617EA0EC45429

[80] Fiebig, J., Divinski, S., Rösner, H., Estrin, Y., & Wilde, G. (2011). Diffusion of Ag and Co in ultrafine-grained α-Ti deformed by equal channel angular pressing. Journal of Applied Physics, 110(8). https://pubs.aip.org/aip/jap/article/110/8/083514/954130

[81] Shousha, S., Kadambi, S. B., Beeler, B., & Kombaiah, B. (2024). Vacancy-mediated transport and segregation tendencies of solutes in fcc nickel under diffusional creep: A density functional theory study. Physical Review Materials, 8(8), 083605. https://journals.aps.org/prmaterials/abstract/10.1103/PhysRevMaterials.8.083605

[82] Morgado, F. F., Katnagallu, S., Freysoldt, C., Klaes, B., Vurpillot, F., Neugebauer, J., ... & Stephenson, L. T. (2021). Revealing atomic-scale vacancy-solute interaction in nickel. Scripta Materialia, 203, 114036. https://www.sciencedirect.com/science/article/pii/S135964622100316X

[83] Magri, M., Lemoine, G., Adam, L., & Segurado, J. (2020). A coupled model of diffusional creep of polycrystalline solids based on climb of dislocations at grain boundaries. Journal of the Mechanics and Physics of Solids, 135, 103786. https://www.sciencedirect.com/science/article/pii/S002250961930732X

[84] Zhang, X., Divinski, S. V., & Grabowski, B. (2022). Ab initio prediction of vacancy energetics in HCP Al-Hf-Sc-Ti-Zr high entropy alloys and the subsystems. Acta Materialia, 227, 117677. https://www.sciencedirect.com/science/article/pii/S1359645422000647

[85] Dobson, D. P., Lindsay-Scott, A., Hunt, S. A., Bailey, E., Wood, I. G., Brodholt, J. P., ... & Wheeler, J. (2019). Anisotropic diffusion creep in postperovskite provides a new model for deformation at the core - mantle boundary. Proceedings of the National Academy of Sciences, 116(52), 26389-26393. https://www.pnas.org/doi/abs/10.1073/pnas.1914826116

[86] Ghosh, S. (2024). Theory and Applications of the Eshelby Ellipsoidal Elastic Inclusion Problem. https://engrxiv.org/preprint/view/4198

[87] Rösler, J., Harders, H., and Bäker, M. (2007). Mechanical behaviour of engineering materials: metals, ceramics, polymers, and composites. Springer Science and Business Media. https://link.springer.com/book/10.1007/978-3-540-73448-2

[88] Ree, J. H. (1994). Grain boundary sliding and development of grain boundary openings in experimentally deformed octachloropropane. Journal of Structural Geology, 16(3), 403-418. https://www.sciencedirect.com/science/article/abs/pii/0191814194900442

[89] Gifkins, R. (1976). Grain-boundary sliding and its accommodation during creep and superplasticity. Metallurgical transactions a, 7, 1225-1232. https://link.springer.com/article/10.1007/BF02656607
[90] Yang, H., Gavras, S., and Dieringa, H. (2021). Creep characteristics of metal matrix composites. In *Encyclopedia of Materials: Composites* (Vol. 1, pp. 375-388). Elsevier. https://www.sciencedirect.com/science/article/abs/pii/B9780128035818118223?via%3Dihub

[91] Adams, M. A., and Murray, G. T. (1962). Direct Observations of Grain-Boundary Sliding in Bi-Crystals of Sodium Chloride and Magnesia. Journal of Applied Physics, 33(6), 2126-2131. https://pubs.aip.org/aip/jap/article/33/6/2126/163641/Direct-Observations-of-Grain-Boundary-Sliding-in

[92] Naziri, H., Pearce, R., Brown, M. H., and Hale, K. F. (1975). Microstructural-mechanism relationship in the zinc/aluminium eutectoid superplastic alloy. Acta Metallurgica, 23(4), 489-496. https://www.sciencedirect.com/science/article/pii/0001616075900887

[93] Sergueeva, A. V., Mara, N. A., and Mukherjee, A. K. (2007). Grain boundary sliding in nanomaterials at elevated temperatures. Journal of materials science, 42, 1433-1438. https://link.springer.com/article/10.1007/s10853-006-0697-0

[94] Zhang, X., Li, W., Ma, J., Li, Y., Zhang, X., and Zhang, X. (2021). Modeling the effects of grain boundary sliding and temperature on the yield strength of high strength steel. Journal of Alloys and Compounds, 851, 1567-1577. https://www.sciencedirect.com/science/article/pii/S092583882033111X

[95] Mikhaylovskaya, A. V., Yakovtseva, O. A., and Irzhak, A. V. (2022). The role of grain boundary sliding and intragranular deformation mechanisms for a steady stage of superplastic flow for Al-Mg-based alloys. Materials Science and Engineering: A, 833, 1425-1438. https://www.sciencedirect.com/science/article/pii/S0921509321017846

[96] Wright, P. K. (1978). The high temperature creep behavior of doped tungsten wire. *Metallurgical Transactions A*, 9, 955-963. https://link.springer.com/article/10.1007/BF02649840

[97] Raj, R., and King, G. W. (1978). Life prediction of tungsten filaments in incandescent lamps. *Metallurgical Transactions A*, 9, 941-946. https://link.springer.com/article/10.1007/BF02649838

[98] Schade, P. (2010). 100 years of doped tungsten wire. *International Journal of Refractory Metals* and *Hard Materials*, 28(6), 648-660. https://www.sciencedirect.com/science/article/pii/S0263436810000752

[99] Rosato, M. G., and Rosato, D. V. (Eds.). (2013). Plastics design handbook. Springer Science and Business Media. https://www.goodreads.com/book/show/6094734-plastics-design-handbook

[100] McCrum, N. G., Buckley, C. P., and Bucknall, C. B. (1997). Principles of polymer engineering. Oxford University Press. https://global.oup.com/academic/product/principles-of-polymer-engineering-9780198565260?cc=in&lang=en&

[101] Ozyhar, T., Hering, S., and Niemz, P. (2013). Viscoelastic characterization of wood: Time dependence of the orthotropic compliance in tension and compression. *Journal of Rheology*, 57(2), 699-717. https://pubs.aip.org/sor/jor/article/57/2/699/241100

[102] Jiang, J., Erik Valentine, B., Lu, J., and Niemz, P. (2016). Time dependence of the orthotropic compression Young's moduli and Poisson's ratios of Chinese fir wood. *Holzforschung*, 70(11), 1093-1101. https://www.degruyterbrill.com/document/doi/10.1515/hf-2016-0001/html

[103] McLean, D. (1966). The physics of high temperature creep in metals. *Reports on Progress in Physics*, 29(1), 1. https://iopscience.iop.org/article/10.1088/0034-4885/29/1/301
[104] Pineau, A., McDowell, D. L., Busso, E. P., and Antolovich, S. D. (2016). Failure of metals II: Fatigue. Acta Materialia, 107, 484-507. https://www.sciencedirect.com/science/article/pii/S135964541500381X?via%3Dihub

[105] Chen, Z., Yang, F., Liu, S., Hu, X., Liu, C., Zhou, Z., ... and Liu, L. (2022). Creep behavior of intermetallic compounds at elevated temperatures and its effect on fatigue life evaluation of Cu pillar bumps. Intermetallics, 144, 107526. https://www.sciencedirect.com/science/article/pii/S096697952200067X?via%3Dihub

[106] Pollock, T. M., and Tin, S. (2006). Nickel-based superalloys for advanced turbine engines: chemistry, microstructure and properties. Journal of propulsion and power, 22(2), 361-374. https://arc.aiaa.org/doi/10.2514/1.18239

[107] Clemens, H., and Mayer, S. (2013). Design, processing, microstructure, properties, and applications of advanced intermetallic TiAl alloys. Advanced engineering materials, 15(4), 191-215. https://advanced.onlinelibrary.wiley.com/doi/full/10.1002/adem.201200231

[108] “Ceiling Collapse in the Interstate 90 Connector Tunnel”. National Transportation Safety Board. Washington, D.C.: NTSB. July 10, 2007. Retrieved 2 December 2016. https://www.ntsb.gov/investigations/AccidentReports/Reports/HAR0702.pdf

[109] Bažant, Z. P., and Zhou, Y. (2002). Why did the world trade center collapse?—Simple analysis. Journal of Engineering Mechanics, 128(1), 2-6. https://ascelibrary.org/doi/10.1061/%28ASCE%290733-9399%282002%29128%3A1%282%29

[110] Lakes, R. S. (2017). Viscoelastic Solids (1998). CRC press. https://www.taylorfrancis.com/books/mono/10.1201/9781315121369/viscoelastic-solids-1998-roderic-lakes-frank-kulacki

[111] “Is glass liquid or solid?”. University of California, Riverside. Retrieved 2008-10-15. https://math.ucr.edu/home/baez/physics/General/Glass/glass.html

[112] Abuzeid, O. M., Al-Rabadi, A. N., and Alkhaldi, H. S. (2011). Recent Advancements in Fractal Geometric-Based Nonlinear Time Series Solutions to the Micro-Quasistatic Thermoviscoelastic Creep for Rough Surfaces in Contact. Mathematical Problems in Engineering, 2011(1), 691270. https://onlinelibrary.wiley.com/doi/10.1155/2011/691270

[113] Long, H., Mao, S., Liu, Y., Zhang, Z., and Han, X. (2018). Microstructural and compositional design of Ni-based single crystalline superalloys—A review. Journal of Alloys and Compounds, 743, 203-220. https://www.sciencedirect.com/science/article/pii/S0925838818302263?via%3Dihub

[114] Suzuki, A., Inui, H., Pollock, T.M. (2015). L12-Strengthened Cobalt-Base Superalloys, Annual Review of Materials Research, 45, 345-368, https://doi.org/10.1146/annurev-matsci-070214-021043, https://www.annualreviews.org/content/journals/10.1146/annurev-matsci-070214-021043

[115] Pelleg, J., and Pelleg, J. (2017). Creep in ceramics (pp. 41-61). Springer International Publishing. https://link.springer.com/book/10.1007/978-3-319-50826-9

[116] Bakunov, V. S., and Belyakov, A. V. (2000). Creep and structure of ceramics. Inorganic materials, 36, 1297-1301. https://link.springer.com/article/10.1023/A:1026658404494

[117] Duddu, R., and Waisman, H. (2012). A temperature dependent creep damage model for polycrystalline ice. Mechanics of Materials, 46, 23-41. https://www.sciencedirect.com/science/article/pii/S0167663611002122?via%3Dihub
[118] Ghosh, S. (2025). Rate-Dependent Plastic Deformation Model of Euler-Bernoulli Beams. https://engrxiv.org/preprint/view/4719

[119] Pandey, M. C., Taplin, D. M. R., Ashby, M. F., and Dyson, B. F. (1986). The effect of prior exposure-time on air-environment/creep interactions. Acta Metallurgica, 34(11), 2225-2233. https://www.sciencedirect.com/science/article/pii/0001616086901689

[120] Neville, A. M. (1971). Creep of concrete: plain, reinforced, and prestressed. https://trid.trb.org/View/99140

[121] Neville, A. M. (1964). Creep of concrete as a function of its cement paste content. Magazine of concrete Research, 16(46), 21-30. https://www.emerald.com/jmacr/article-abstract/16/46/21/414580/Creep-of-concrete-as-a-function-of-its-cement?redirectedFrom=fulltext

[122] Bažant, Z. P., and Osman, E. (1976). Double power law for basic creep of concrete. Matériaux et Construction, 9, 3-11. https://link.springer.com/article/10.1007/BF02478522

[123] Yu, Q., Bazant, Z. P., and Wendner, R. (2012). Improved algorithm for efficient and realistic creep analysis of large creep-sensitive concrete structures. ACI Structural Journal, 109(5), 665. http://cee.northwestern.edu/people/bazant/PDFs/Papers/515.pdf

[124] Ross, A. D. (1958, March). Creep of concrete under variable stress. In Journal Proceedings (Vol. 54, No. 3, pp. 739-758). https://www.concrete.org/publications/internationalconcreteabstractsportal.aspx?m=details&id=11466

[125] Bissonnette, B., Pigeon, M., and Vaysburd, A. M. (2007). Tensile creep of concrete: study of its sensitivity to basic parameters. ACI Materials journal, 104(4), 360. https://www.concrete.org/publications/internationalconcreteabstractsportal.aspx?m=details&ID=18825

[126] Ranaivomanana, N., Multon, S., and Turatsinze, A. (2013). Basic creep of concrete under compression, tension and bending. Construction and Building Materials, 38, 173-180. https://www.sciencedirect.com/science/article/pii/S0950061812006095

[127] Orozco-Caballero, A., Lunt, D., Robson, J. D., & Da Fonseca, J. Q. (2017). How magnesium accommodates local deformation incompatibility: a high-resolution digital image correlation study. Acta Materialia, 133, 367-379. https://www.sciencedirect.com/science/article/pii/S1359645417304275

[128] Orozco-Caballero, A., Jackson, T., & Da Fonseca, J. Q. (2021). High-resolution digital image correlation study of the strain localization during loading of a shot-peened RR1000 nickel-based superalloy. Acta Materialia, 220, 117306. https://www.sciencedirect.com/science/article/pii/S1359645421006868

[129] Singh, P. S., Liang, Z., Pharr, G. M., & de Boer, M. P. (2020). Creep of a thermally stable nanocrystalline nickel tungsten alloy as measured by high temperature nanoindentation. Materials Science and Engineering: A, 784, 139309. https://www.sciencedirect.com/science/article/pii/S0921509320303919

[130] Yagi, N., Rikukawa, A., Mizubayashi, H., & Tanimoto, H. (2006). Experimental tests of the elementary mechanism responsible for creep deformation in nanocrystalline gold. Physical Review B—Condensed Matter and Materials Physics, 74(14), 144105. https://journals.aps.org/prb/abstract/10.1103/PhysRevB.74.144105
[131] Rozman, K. A., Detrois, M., Liu, T., Gao, M. C., Jablonski, P. D., & Hawk, J. A. (2020). Long-term creep behavior of a CoCrFeNiMn high-entropy alloy. Journal of Materials Engineering and Performance, 29(9), 5822-5839. https://link.springer.com/article/10.1007/s11665-020-05103-2

[132] Xing, B., Zou, W., Rupert, T. J., & Cao, P. (2024). Vacancy diffusion barrier spectrum and diffusion correlation in multicomponent alloys. Acta Materialia, 266, 119653. https://www.sciencedirect.com/science/article/pii/S1359645424000065

[133] Xu, R., Chen, C. C., Wu, L., Scott, M. C., Theis, W., Ophus, C., ... & Miao, J. (2015). Three-dimensional coordinates of individual atoms in materials revealed by electron tomography. Nature materials, 14(11), 1099-1103. https://www.nature.com/articles/nmat4426

[134] Xu, C., & Was, G. S. (2013). In situ proton irradiation creep of ferritic–martensitic steel T91. Journal of nuclear materials, 441(1-3), 681-687. https://www.sciencedirect.com/science/article/pii/S0022311513005497

[135] Berry, J., Rottler, J., Sinclair, C. W., & Provatas, N. (2015). Atomistic study of diffusion-mediated plasticity and creep using phase field crystal methods. Physical Review B, 92(13), 134103. https://journals.aps.org/prb/abstract/10.1103/PhysRevB.92.134103

[136] Voyiadjis, G. Z., & Song, Y. (2019). Strain gradient continuum plasticity theories: theoretical, numerical and experimental investigations. International Journal of Plasticity, 121, 21-75. https://www.sciencedirect.com/science/article/pii/S0749641918307344

[137] Voyiadjis, G. Z., & Faghihi, D. (2012). Thermo-mechanical strain gradient plasticity with energetic and dissipative length scales. International Journal of Plasticity, 30, 218-247. https://www.sciencedirect.com/science/article/pii/S074964191100177X

[138] Khalajhedayati, A., & Rupert, T. J. (2015). High-temperature stability and grain boundary complexion formation in a nanocrystalline Cu-Zr alloy. Jom, 67(12), 2788-2801. https://link.springer.com/article/10.1007/s11837-015-1644-9

[139] Sendek, A. D., Cubuk, E. D., Antoniuk, E. R., Cheon, G., Cui, Y., & Reed, E. J. (2018). Machine learning-assisted discovery of many new solid li-ion conducting materials. arXiv preprint arXiv:1808.02470. https://arxiv.org/abs/1808.02470

[140] Ghosh, S. (2025). Rate-Independent Gradient-Enhanced Plastic Deformation Model of Euler-Bernoulli Beams. https://engrxiv.org/preprint/view/4718

[141] Gurtin, M. E. (1996). Generalized Ginzburg-Landau and Cahn-Hilliard equations based on a microforce balance. Physica D: Nonlinear Phenomena, 92(3-4), 178-192. https://www.sciencedirect.com/science/article/pii/0167278995001735

[142] Gurtin, M. E., Fried, E., & Anand, L. (2010). The mechanics and thermodynamics of continua. Cambridge university press. https://books.google.com/books?hl=en&lr=&id=eGUQQaDsTsQC&oi=fnd&pg=PR5&dq=Gurtin,+M.+E.,+Fried,+E.,+%5C%26+Anand,+L.+ (2010).+The+mechanics+and+thermodynamics+of+continua.+Cambridge+university+ press.&ots=2ct4rX-69r&sig=jSEjyBQm_AUAN3dRiICmPjgoTnw

[143] Geers, M. G. D., Cottura, M., Appolaire, B., Busso, E. P., Forest, S., & Villani, A. (2014). Coupled glide-climb diffusion-enhanced crystal plasticity. Journal of the Mechanics and Physics of Solids, 70, 136-153. https://www.sciencedirect.com/science/article/pii/S0022509614000908
[144] Gibson, J. S. L., Schröders, S., Zehnder, C., & Korte-Kerzel, S. (2017). On extracting mechanical properties from nanoindentation at temperatures up to 1000 C. Extreme Mechanics Letters, 17, 43-49. https://www.sciencedirect.com/science/article/pii/S2352431617300925

[145] Bergers, L. I. J. C., Hoefnagels, J. P. M., & Geers, M. G. D. (2011, May). Creep measurements in free-standing thin metal film micro-cantilever bending. In MEMS and Nanotechnology, Volume 4: Proceedings of the 2011 Annual Conference on Experimental and Applied Mechanics (pp. 167-171). New York, NY: Springer New York. https://link.springer.com/chapter/10.1007/978-1-4614-0210-7_24

[146] Petkov, M., Chevalier, M., Dean, D., & Cocks, A. C. (2021). Creep-fatigue interactions in a polycrystalline structural material under typical high-temperature power plant operating conditions. arXiv preprint arXiv:2103.00320. https://arxiv.org/abs/2103.00320

[147] Wallis, D., Hansen, L. N., Wilkinson, A. J., & Lebensohn, R. A. (2021). Dislocation interactions in olivine control postseismic creep of the upper mantle. Nature Communications, 12(1), 3496. https://www.nature.com/articles/s41467-021-23633-8

[148] Caillard, D., Rautenberg, M., & Feugas, X. (2015). Dislocation mechanisms in a zirconium alloy in the high-temperature regime: An in situ TEM investigation. Acta Materialia, 87, 283-292. https://www.sciencedirect.com/science/article/pii/S1359645415000208

[149] Hirth, G. (2002). Laboratory constraints on the rheology of the upper mantle. Reviews in Mineralogy and Geochemistry, 51(1), 97-120. https://pubs.geoscienceworld.org/msa/ring/article-abstract/51/1/97/87437

[150] Beyerlein, I. J., Li, Z., & Mara, N. A. (2022). Mechanical properties of metal nanolaminates. Annual Review of Materials Research, 52, 281-304. https://www.annualreviews.org/content/journals/10.1146/annurev-matsci-081320-031236

[151] Makineni, S. K., Kumar, A., Lenz, M., Kontis, P., Meiners, T., Zenk, C., ... & Gault, B. (2018). On the diffusive phase transformation mechanism assisted by extended dislocations during creep of a single crystal CoNi-based superalloy. Acta Materialia, 155, 362-371. https://www.sciencedirect.com/science/article/pii/S1359645418304713

[152] Lilensten, L., Antonov, S., Gault, B., Tin, S., & Kontis, P. (2021). Enhanced creep performance in a polycrystalline superalloy driven by atomic-scale phase transformation along planar faults. Acta Materialia, 202, 232-242. https://www.sciencedirect.com/science/article/pii/S1359645420308600

[153] Mosquera-Lois, I., Kavanagh, S. R., Klarbring, J., Tolborg, K., & Walsh, A. (2023). Imperfections are not 0 K: free energy of point defects in crystals. Chemical Society Reviews, 52(17), 5812-5826. https://pubs.rsc.org/en/content/articlehtml/2012/zb/d3cs00432e

[154] Paladino, A. E., & Coble, R. L. (1963). Effect of grain boundaries on diffusion-controlled processes in aluminum oxide. Journal of the American Ceramic Society, 46(3), 133-136. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1963.tb11696.x

[155] Ashby, M. F., & Verrall, R. A. (1973). Diffusion-accommodated flow and superplasticity. Acta metallurgica, 21(2), 149-163. https://www.sciencedirect.com/science/article/pii/0001616073900576

[156] Langdon, T. G. (1994). A unified approach to grain boundary sliding in creep and superplasticity. Acta metallurgica et materialia, 42(7), 2437-2443. https://www.sciencedirect.com/science/article/pii/0956715194903220
[157] Yokogawa, K., Fukuyama, S., Kudo, K., & Shewmon, P. G. (1989). Effect of hydrogen attack on tensile and creep properties of low carbon steel. International journal of pressure vessels and piping, 37(5), 365-385. https://www.sciencedirect.com/science/article/pii/S0308016189900306

[158] Shewmon, P. (2016). Thermo-and electro-transport in solids. In Diffusion in solids (pp. 223-241). Cham: Springer International Publishing. https://link.springer.com/content/pdf/10.1007/978-3-319-48206-4_7?pdf=chapter%20toc

[159] Ghahremani, F. (1980). Effect of grain boundary sliding on anelasticity of polycrystals. International Journal of Solids and Structures, 16(9), 825-845. https://www.sciencedirect.com/science/article/pii/S0020768380900529

[160] Ruano, O. A., & Sherby, O. D. (1982). Low stress creep of fine-grained materials at intermediate temperatures: Diffusional creep or grain boundary sliding?. Materials Science and Engineering, 56(2), 167-175. https://www.sciencedirect.com/science/article/pii/S0025541682901690

[161] Lessing, P. A., & Gordon, R. S. (1977). Creep of polycrystalline alumina, pure and doped with transition metal impurities. Journal of Materials Science, 12(11), 2291-2302. https://link.springer.com/article/10.1007/BF00552251

[162] Wakai, F., Nagano, T., & Iga, T. (1997). Hardening in creep of alumina by zirconium segregation at the grain boundary. Journal of the American Ceramic Society, 80(9), 2361-2366. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1997.tb03128.x

[163] Nix, W. D. (1988). Mechanisms and controlling factors in creep fracture. Materials Science and Engineering: A, 103(1), 103-110. https://www.sciencedirect.com/science/article/pii/S0025541688905563

[164] Kassner, M. E., & Pérez-Prado, M. T. (2000). Five-power-law creep in single phase metals and alloys. Progress in materials science, 45(1), 1-102. https://www.sciencedirect.com/science/article/pii/S0079642599000067

[165] Mohamed, F. A., & Langdon, T. G. (1974). The transition from dislocation climb to viscous glide in creep of solid solution alloys. Acta metallurgica, 22(6), 779-788. https://www.sciencedirect.com/science/article/pii/S0001616074900881

[166] Maji, M., Eswaran, K. S., Ghosh, S., Seshasayanan, K., & Shukla, V. (2023). Equivalence of nonequilibrium ensembles: Two-dimensional turbulence with a dual cascade. Physical Review E, 108(1), 015102.

[167] Langdon, T. G. (1977). The relationship between strain rate sensitivity and ductility in superplastic materials. Scripta Metallurgica, 11(11), 997-1000. https://www.sciencedirect.com/science/article/pii/S003697487790254X

[168] Mohamed, F. A., & Li, Y. (2001). Creep and superplasticity in nanocrystalline materials: current understanding and future prospects. Materials Science and Engineering: A, 298(1-2), 1-15. https://www.sciencedirect.com/science/article/pii/S0928493100001909

[169] Atkinson, A. (1988). Interfacial Diffusion. MRS Online Proceedings Library, 122(1), 183-192. https://link.springer.com/article/10.1557/PROC-122-183

[170] Herwegh, M., & Jenni, A. (2001). Granular flow in polymineralic rocks bearing sheet silicates: new evidence from natural examples. Tectonophysics, 332(3), 309-320. https://www.sciencedirect.com/science/article/pii/S0040195100002882
[171] Hirth, G., & Kohlstedt, D. (2003). Rheology of the upper mantle and the mantle wedge: A view from the experimentalists. Geophysical monograph-american geophysical union, 138, 83-106. http://www.soest.hawaii.edu/GG/FACULTY/smithkonter/GG631/other/HirthKohlstedt_2000.pdf

[172] Wang, Z., Gu, L., Zhang, Q., Yue, S., & Zhang, G. (2020). Creep characteristics and prediction of creep failure of rock discontinuities under shearing conditions. International Journal of Earth Sciences, 109(3), 945-958. https://link.springer.com/article/10.1007/s00531-020-01842-8

[173] Tasaka, M., Zimmerman, M. E., Kohlstedt, D. L., Stünitz, H., & Heilbronner, R. (2017). Rheological weakening of olivine+ orthopyroxene aggregates due to phase mixing: Part 2. Microstructural development. Journal of Geophysical Research: Solid Earth, 122(10), 7597-7612. https://agupubs.onlinelibrary.wiley.com/doi/abs/10.1002/2017jb014311

[174] Tasaka, M., Zimmerman, M. E., & Kohlstedt, D. L. (2017). Rheological weakening of olivine+ orthopyroxene aggregates due to phase mixing: 1. Mechanical behavior. Journal of Geophysical Research: Solid Earth, 122(10), 7584-7596. https://agupubs.onlinelibrary.wiley.com/doi/abs/10.1002/2017JB014333

[175] Ghosh, S., Kumawat, K., Sajish, S. D., Arul, J., & Bhattacharya, B. (2025). Time-dependent fatigue reliability of main vessel steel structural components in sodium cooled fast breeder reactors. Nuclear Engineering and Design, 433, 113820. https://www.sciencedirect.com/science/article/pii/S0029549324009208

[176] Hansen, L. N., Zimmerman, M. E., & Kohlstedt, D. L. (2011). Grain boundary sliding in San Carlos olivine: Flow law parameters and crystallographic-preferred orientation. Journal of Geophysical Research: Solid Earth, 116(B8). https://agupubs.onlinelibrary.wiley.com/doi/abs/10.1029/2011jb008220

[177] Goldsby, D. L., & Kohlstedt, D. L. (2001). Superplastic deformation of ice: Experimental observations. Journal of Geophysical Research: Solid Earth, 106(B6), 11017-11030. https://agupubs.onlinelibrary.wiley.com/doi/abs/10.1029/2000jb900336

[178] Goldsby, D. L., & Kohlstedt, D. L. (1997). Grain boundary sliding in fine-grained ice I. Scripta Materialia, 37(9), 1399-1406. https://citeseerx.ist.psu.edu/document?repid=rep1&type=pdf&doi=549d7611a760e4c4aa06b9180573bdf3accc32ca

[179] Bürgmann, R., & Dresen, G. (2008). Rheology of the lower crust and upper mantle: Evidence from rock mechanics, geodesy, and field observations. Annu. Rev. Earth Planet. Sci., 36(1), 531-567. https://www.annualreviews.org/content/journals/10.1146/annurev.earth.36.031207.124326

[180] Mocellin, A., & Kingery, W. D. (1971). Creep Deformation in MgO-Saturated Large-Grain-Size Al2O3. Journal of the American Ceramic Society, 54(7), 339-341. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1971.tb12309.x

[181] Chokshi, A. H. (1990). An evaluation of the grain-boundary sliding contribution to creep deformation in polycrystalline alumina. Journal of materials science, 25(7), 3221-3228. https://link.springer.com/article/10.1007/BF00587678

[182] Heuer, A. H. (2008). Oxygen and aluminum diffusion in α-Al2O3: How much do we really understand?. Journal of the European Ceramic Society, 28(7), 1495-1507. https://www.sciencedirect.com/science/article/pii/S0955221907006097
[183] DIMOS, D., KOHLSTEDI, D., & SCHMALZRIED, H. (1988). High-temperature creep and kiketic demixing in (Co, Mg) O. Journal of the American Ceramic Society, 71(9), 732-741. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1988.tb06406.x

[184] Gifkins, R. C. (1968). Diffusional creep mechanisms. Journal of the American Ceramic Society, 51(2), 69-72. https://ceramics.onlinelibrary.wiley.com/doi/abs/10.1111/j.1151-2916.1968.tb11838.x

[185] Koch, R. H., Lloyd, J. R., & Cronin, J. (1985). 1 f noise and grain-boundary diffusion in aluminum and aluminum alloys. Physical review letters, 55(22), 2487. https://journals.aps.org/prl/abstract/10.1103/PhysRevLett.55.2487

[186] Raj, R. (1975). Transient behavior of diffusion-induced creep and creep rupture. Metallurgical Transactions A, 6(8), 1499. https://link.springer.com/article/10.1007/BF02641961

[187] Raj, R., & Ashby, M. F. (1975). Intergranular fracture at elevated temperature. Acta metallurgica, 23(6), 653-666. https://www.sciencedirect.com/science/article/pii/0001616075900474

[188] Kassner, M. E., & Hayes, T. A. (2003). Creep cavitation in metals. International journal of plasticity, 19(10), 1715-1748. https://www.sciencedirect.com/science/article/pii/S0749641902001110

[189] Meixner, F., Ahmadi, M. R., & Sommitsch, C. (2022). Cavity nucleation and growth in nickel-based alloys during creep. Materials, 15(4), 1495. https://www.mdpi.com/1996-1944/15/4/1495

[190] Fuller Jr, E. R., Fields, R. J., Chuang, T. J., & Singhal, S. (1984). Characterization of creep damage in metals using small angle neutron scattering. JOURNAL OF RESEARCH of the National Bureau of Standards, 89(1), 35. https://pmc.ncbi.nlm.nih.gov/articles/PMC6768172/

[191] Kim, B. N., Morita, K., & Hiraga, K. (2003). Rate of diffusion creep accompanied by grain boundary sliding in elongated microstructures. Materials Science and Engineering: A, 363(1-2), 67-71. https://www.sciencedirect.com/science/article/pii/S0921509303005768

[192] Wang, C. (2010). Study of Deformation Behavior of Nanocrystalline Nickel using Nanoindentation Techniques. https://trace.tennessee.edu/utk_graddiss/862/

[193] Brassard, J. (2003). Deformation mechanisms during creep and cold rolling of nanocrystalline nickel. https://utoronto.scholaris.ca/items/f92e9166-1af4-408c-b8cb-3ada34a894a3

[194] Schiotz, J., Vegge, T., & Jacobsen, K. W. (1998). Atomic-scale modeling of the deformation of nanocrystalline metals. MRS Online Proceedings Library (OPL), 538, 299. https://www.cambridge.org/core/journals/mrs-online-proceedings-library-archive/article/atomicscale-modeling-of-the-deformation-of-nanocrystalline-metals/39D96AE2881B141C423617EA0EC45429

[195] Ghosh, S. (2025). Mathematical Foundations of Deep Learning. https://hal.science/hal-04928560/

[196] Zhang, B. B., Tang, Y. G., Mei, Q. S., Li, X. Y., & Lu, K. (2022). Inhibiting creep in nanograined alloys with stable grain boundary networks. Science, 378(6620), 659-663. https://www.science.org/doi/abs/10.1126/science.abq7739

[197] Carter, C. B., & Norton, M. G. (2007). Ceramic materials: science and engineering (Vol. 716). Springer. https://link.springer.com/book/10.1007/978-1-4614-3523-5
[198] Meyers, M. A., & Chawla, K. K. (2008). Mechanical behavior of materials. Cambridge university press. https://books.google.com/books?hl=en&lr=&id=v_oAwAAQBAJ&oi=fnd&pg=PT19&dq=Meyers,+M.+A.,+%26+Chawla,+K.+K.+ (2008). +Mechanical+behavior+of+materials.+Cambridge+univer-+sity+press.&ots=Kqraxbfqc9&sig=PXrjf2arGJX2qTUik4iQ3sw4egY

[199] Nembach, E. (1997). Particle strengthening of metals and alloys. https://cir.nii.ac.jp/crid/1130000795362721920

[200] Ardell, A. J. (1985). Precipitation hardening. Metallurgical Transactions A, 16(12), 2131-2165. https://link.springer.com/article/10.1007/BF02670416

[201] Reed, R. C. (2008). The superalloys: fundamentals and applications. Cambridge university press. https://dlib.scu.ac.ir/bitstream/Hannan/369808/2/9780521859042.pdf

[202] Tin, S., & Pollock, T. M. (2014). Nickel-Based Superalloys. Turbine Aerodynamics, Heat Transfer, Materials, and Mechanics; American Institute of Aeronautics and Astronautics, Inc.: Reston, VA, USA, 243, 423-466. https://www.academia.edu/download/63407285/Turbine_aerodynamics_Heat_transfer_Materials_and_Mechanics20200523-23383-107shcz.pdf#page=440

[203] Kamaraj, M. (2003). Rafting in single crystal nickel-base superalloys—An overview. Sadhana, 28(1), 115-128. https://link.springer.com/article/10.1007/BF02717129

[204] Abe, F. (2008). Precipitate design for creep strengthening of 9% Cr tempered martensitic steel for ultra-supercritical power plants. Science and Technology of Advanced Materials, 9(1), 013002. https://iopscience.iop.org/article/10.1088/1468-6996/9/1/013002/meta

[205] Danielsen, H. K. (2016). Review of Z phase precipitation in 9-12 wt-Cr steels. Materials Science and Technology, 32(2), 126-137. https://journals.sagepub.com/doi/abs/10.1179/1743284715Y.0000000066

[206] Tkachev, E., Belyakov, A., & Kaibyshev, R. (2020). Creep strength breakdown and microstructure in a 9% Cr steel with high B and low N contents. Materials Science and Engineering: A, 772, 138821. https://www.sciencedirect.com/science/article/pii/S0921509319316065

[207] Abe, F., Taneike, M., & Sawada, K. (2007). Alloy design of creep resistant 9Cr steel using a dispersion of nano-sized carbonitrides. International Journal of Pressure Vessels and Piping, 84(1-2), 3-12. https://www.sciencedirect.com/science/article/pii/S030801610600158X

[208] Balan, A., Perez, M., Chaise, T., Cazottes, S., Bardel, D., Corpace, F., ... & Nelias, D. (2021). Precipitation of γ" in Inconel 718 alloy from microstructure to mechanical properties. Materialia, 20, 101187. https://www.sciencedirect.com/science/article/pii/S2589152921001903

[209] Karnesky, R. A., Meng, L., & Dunand, D. C. (2007). Strengthening mechanisms in aluminum containing coherent Al3Sc precipitates and incoherent Al2O3 dispersoids. Acta Materialia, 55(4), 1299-1308. https://www.sciencedirect.com/science/article/pii/S135964540600718X

[210] Krug, M. E., & Dunand, D. C. (2011). Modeling the creep threshold stress due to climb of a dislocation in the stress field of a misfitting precipitate. Acta materialia, 59(13), 5125-5134. https://www.sciencedirect.com/science/article/pii/S1359645411003004

[211] Rösler, J., & Arzt, E. (1988). The kinetics of dislocation climb over hard particles—I. Climb without attractive particle-dislocation interaction. Acta Metallurgica, 36(4), 1043-1051. https://www.sciencedirect.com/science/article/pii/0001616088901587
[212] Arzt, E., & Rösler, J. (1988). The kinetics of dislocation climb over hard particles—II. Effects of an attractive particle-dislocation interaction. Acta Metallurgica, 36(4), 1053-1060. https://www.sciencedirect.com/science/article/pii/0001616088901599

[213] Rösler, J., & Arzt, E. (1990). A new model-based creep equation for dispersion strengthened materials. Acta metallurgica et Materialia, 38(4), 671-683. https://www.sciencedirect.com/science/article/pii/0956715190902234

[214] Deshmukh, S. P., Mishra, R. S., & Robertson, I. M. (2010). Investigation of creep threshold stresses using in situ TEM straining experiment in an Al-5Y2O3-10SiC composite. Materials Science and Engineering: A, 527(9), 2390-2397. https://www.sciencedirect.com/science/article/pii/S0921509309013185

[215] Arzt, E. (1991). Creep of dispersion strengthened materials: a critical assessment. https://publikationen.sulb.uni-saarland.de/handle/20.500.11880/24031

[216] Maruyama, K., Sawada, K., & Koike, J. I. (2001). Strengthening mechanisms of creep resistant tempered martensitic steel. ISIJ international, 41(6), 641-653. https://www.jstage.jst.go.jp/article/isijinternational1989/41/6/41_6_641/_article/-char/ja/

[217] Rabotnov, Y. N. (1969). Creep rupture. In Proceedings of the 12th International Congress on Applied Mechanics (pp. 342-349).

[218] Kachanov, L. M. (1958). Time of rupture process under creep conditions. Izv. Akad. Nauk SSSR. Otd. Tekh. Nauk, 8, 26-31.

[219] Dyson, B. F. (1988). Continuum damage mechanics models for creep. Metallurgical Transactions A, 19(6), 1389-1395.

[220] Lemaitre, J. (1985). A continuous damage mechanics model for ductile fracture. Journal of Engineering Materials and Technology, 107(1), 83-89.

[221] Chaboche, J. L. (1981). Continuum damage mechanics: Part I-General concepts. Journal of Applied Mechanics, 48(2), 364-368.

[222] Chaboche, J. L. (1988). Continuum damage mechanics: Part II-Damage growth, crack initiation, and crack growth. Journal of Applied Mechanics, 55(1), 65-72.

[223] Hayhurst, D. R. (1972). Creep rupture under multi-axial states of stress. Journal of the Mechanics and Physics of Solids, 20(6), 381-382.

[224] Tvergaard, V., & Needleman, A. (1984). Analysis of the cup-cone fracture in a round tensile bar. Acta Metallurgica, 32(1), 157-169.

[225] Needleman, A. (1987). A continuum model for void nucleation by inclusion debonding. Journal of Applied Mechanics, 54(3), 525-531.

[226] Murakami, S. (1988). Mechanical modeling of material damage. Journal of Applied Mechanics, 55(2), 280-286.

[227] Shenoy, M., & McMeeking, R. J. (2010). Multiscale modeling of creep-damage by grain boundary cavitation. Acta Materialia, 58(13), 4424-4438.

[228] Cailletaud, G., & Sai, L. (2012). Multiscale approaches to creep and fatigue damage. International Journal of Plasticity, 32, 17-30.

[229] Pettinari-Sturmel, P., & Vincent, R. (2016). Oxidation-creep interactions in high-temperature alloys. Corrosion Science, 104, 52-61.
[230] Gurson, A. L. (1977). Continuum theory of ductile rupture by void nucleation and growth. *Journal of Engineering Materials and Technology*, 99(1), 2–15.

[231] Skelton, R. P., & Hayhurst, D. R. (1987). Creep damage mechanics: The effect of multiaxial stress states on the creep rupture of notched bars. *Journal of the Mechanics and Physics of Solids*, 35(4), 281–296.

[232] Miller, W. S., & McDowell, D. L. (1992). Creep damage mechanics: A review. *Journal of Engineering Materials and Technology*, 114(3), 257–265.

[233] de Borst, R., & Pamin, J. (1996). Gradient plasticity in numerical simulation of concrete cracking. *European Journal of Mechanics - A/Solids*, 15(3), 295–320.

[234] Ainsworth, R. A. (Ed.). (2003). *Assessment Procedure for the High Temperature Response of Structures*. Issue 3. Barnwood: BEGL Ltd.

[235] Hyde, C. J., Hyde, T. H., Sun, W., & Becker, A. A. (2010). Damage mechanics based predictions of creep crack growth in 316 stainless steel. *Engineering Fracture Mechanics*, 77(12), 1965–1982.

[236] Gonzalez, J. M., & Ruggieri, N. (2004). Micro–macro creep damage simulation for welded joints. *International Journal of Pressure Vessels and Piping*, 81(5), 353–363.

[237] Rao, P. S., & Reddy, B. V. (2011). Creep damage analysis of mod.9Cr-1Mo steel welds considering strain softening and damage due to void formation. *International Journal of Pressure Vessels and Piping*, 88(4), 201–210.

[238] Hayhurst, D. R. (1990). Multi-axial creep rupture of a model structure using a two-parameter material model. *International Journal of Mechanical Sciences*, 32(1), 35–48.